Toward Enabling Spatial Control of Ti-6Al-4V Solidification
Microstructure in the Electron Beam Melting Process Sneha P. Narra, Ross Cunningham, Daniel Christiansen, Jack Beuth and Anthony D. Rollett
Department of Mechanical Engineering, Carnegie Mellon Univ., Pittsburgh, PA 15213
Material Science and Engineering Department, Carnegie Mellon Univ., Pittsburgh, PA 15213
Abstract In this work, relationships between prior beta grain size in solidified Ti-6Al-4V and melting
process parameters in the Arcam Electron Beam Melting (EBM) process are investigated. Toward
this goal, samples are built on an Arcam S12 machine at Carnegie Mellon University by
specifically varying the Arcam proprietary speed function and beam current over process space
for a variety of test specimens. Optical microscopy is used to measure the prior beta grain widths
and assess the number of prior beta grains present in a melt pool in the raster region of the build.
Results demonstrate that the number of grains across the width of a bead is constant for a fixed
deposition geometry. The resulting understanding of the relationship between primary machine
variables and prior beta grain widths is a key step toward understanding and enabling the spatial
control of as-built microstructure in the EBM process.
Introduction Electron beam powder bed Additive Manufacturing (AM) is attractive due to its working
conditions, e.g. elevated build temperature and a vacuum build environment, which help
manufacture residual-stress-free and contamination-free components . In addition, high beam
powers and efficient transfer of power into the part yield high deposition rates and facilitate
building of components from materials with high melting points up to 3500C . In this work Ti-
6Al-4V (Ti64) is the material of interest owing to its extensive applications in the aerospace
industry and also the availability of well-established control themes on the Arcam Electron Beam
Melting (EBM) machine .
It is critical to know the mechanical behavior of AM as-built components to qualify them for use
in industrial applications. This motivates this study of the effect of process variables on Ti64
solidification microstructure, which governs some mechanical properties of the end part . At
the same time, it is important to maintain or improve other process outcomes such as process
precision and build rate, which are governed directly or indirectly by melt pool geometry. Hence,
it is important to understand the integrated control of melt pool geometry and solidification
microstructure. Toward this goal, techniques have been developed for integrated control of melt
pool geometry and microstructure of Ti64 in an Electron Beam Wire Feed Process (EBF3) and in
EBM for single bead geometries  . Using these concepts of prior beta grain width control
shown in Figure 1, in this work, beta grain width is varied by controlling the melt pool geometry
using the primary beam parameters in the EBM process. Other previous work has explored the
microstructure in Ti64 EBM deposits by describing the evolution of microstructure, mechanical
properties and their dependence on part dimensions, build orientation, and location   . This
work focuses primarily on prior beta grain width control as a first step toward enabling full
microstructure control in fabricated components using EBM machine process parameters. To the
knowledge of the authors, this work is unique and it allows any EBM user with basic (Level 1)
machine training to control prior beta grain widths in the raster regions of bulky as-built parts.
Microstructure generally affects mechanical properties and, unlike the alpha lath microstructure,
it is difficult to modify as-built prior beta grain size through post-processing heat treatments 
. Prior beta grain size is mainly controlled by the rate at which the melt pool cools down from
the melting temperature to the beta transus temperature during the process. This scales with the
thermal conditions at the start of solidification, that is, the thermal gradient and resulting cooling
rate at the solidus temperature, which in turn varies with the primary process parameters i.e. beam
current and travel speed .
Arcam Electron Beam Melting Process
Primary variables for beam control in the EBM process are beam speed, beam current, and focus
offset as shown in Figure 2. When a part is built in the automatic mode, beam current is changed
with part height based on a thermal model in the machines control software and speed is controlled
by the variable speed function. Focus offset controls the spot size of the electron beam. In this
work, the effect of focus offset is not discussed in detail and it is not methodically varied across
its operating range. Focus offset is not expected to have a significant effect on beta grain size. The
speed function is a proprietary variable and an initial study was performed to understand the role
of this variable during the melting process. Mahale  discussed the variation of beam current
and travel speed with part height for various speed function and layer thickness values. Using that
data, lines of constant speed function (Figure 3) have been developed in power and velocity space.
Qualitative analysis of the data plotted in Figure 3 shows that curves of constant speed function
have a similar trend to curves of constant melt pool area in Figure 1 from the previous work 
 done on single bead tests in the Arcam EBM process. Therefore, we can say that, based on
Figure 1: Plots showing integrated solidification microstructure and melt pool geometry
control for Ti64 single beads during the electron beam melting process .
the beam current, the speed function changes beam travel velocity in an attempt to maintain
constant melt pool geometry throughout the build process. As a part of this work, experiments
have been performed to establish a quantitative relationship between speed function and melt pool
geometry which was then used to understand and control the prior beta grain width in solid blocks.
Single Bead Tests
No-added-powder single bead tests have been
performed for different speed function and beam current combinations as listed in Table 1 on an
Arcam S12 machine at Carnegie Mellon University. In these tests, there was no powder on the
Ti64 plate. The beam carrying a specified current and operating at a given speed function traveled
from one end of the plate to the other leaving rectangular melt tracks as shown in Figure 4. The
plate base was maintained at a temperature of approximately 750C.
Figure 4: Image of the Ti64 plate with single bead melt tracks.
Figure 2: Photograph showing the primary
beam variables on the Arcam machine.
Figure 3: Plot demonstrating the effect of beam
current and velocity (speed function).
Table 1: Parameter set used for the no-added-powder single bead experiments.
Sample No. Beam Current mA Speed Function Focus Offset mA
1 (Nominal) 17 36 19
2 17 17 19
3 17 7 19
4 17 75 19
5 17 154 19
6 8.5 36 19
7 8.5 17 19
8 34 36 19
9 34 17 19
10 12 30 0
11 12 13 0
12 12 4 0
13 12 64 0
14 12 130 0
15 6 30 0
16 6 13 0
17 24 30 0
18 24 13 0
Multi-Layer Blocks (or Solid Builds)
Figure 5 shows the experimental layout of 9 multi-layer
blocks of dimensions 30W30L20H mm built by varying speed function and beam current in the build theme (shown
in Figure 6) while holding other melting parameters
constant. This was done for both contour and bulk raster
regions, though results are presented only for bulk raster
regions in this study. From Table 2, it can be seen that out
of 9 samples, 5 samples were built with varying speed
function at a constant beam current. The remaining 4
samples were built with varying beam current at constant
speed function. Sample 1 was built using nominal build
conditions for the Ti64 alloy.
Experimental Results and Analysis
Single Bead Tests
Single bead melt lines were sectioned along the transverse direction of the melt track at locations
well away from the plate edges, where the melt pool reaches steady-state conditions. Samples were
mounted, polished and etched using Krolls reagent . Images were taken using an Alicona
InfiniteFocus optical microscope.
Figure 5: Layout for multi-layer block
Figure 6: Image showing various parameters on
the machine that control the melting process.
Table 2: Parameters for multi-layer block experiments.
An example of a melt pool cross-section image used
for analysis is shown in Figure 7. The melt pool is
marked along the solidification boundary, which is
where the morphology is different from the start
plate. The melt pool dimensions of cross-sectional
area, width and depth were measured. Grains grew
from the melt pool boundary upward and toward the
center and, qualitatively, a majority of the grains
appear to be columnar. Samples 4, 5 and 8 had melt
pools that were very shallow and made it difficult to
mark the boundaries.